2Metal Matrix Composites (MMC) Metal matrix composites (MMCs), as the name implies, have a metal matrix. Examples of matrices in such composites include aluminum, magnesium, and titanium.Typical ﬁbers include carbon and silicon carbide.Metals are mainly reinforced to increase or decrease their properties to suit the needs of design. For example, the elastic stiffness and strength of metals can be increased, and large coefﬁcients of thermal expansion and thermal and electric conductivities of metals can be reduced, by the addition of ﬁbers such as silicon carbide.
3Advantages of MMC’sMetal matrix composites are mainly used to provide advantages over monolithic metals such as steel and aluminum. These advantages include higher speciﬁc strength and modulus by reinforcing low-density metals, such as aluminum and titanium; lower coefﬁcients of thermal expansion by reinforcing with ﬁbers with low coefﬁcients of thermal expansion, such as graphite; and maintaining properties such as strength at high temperatures.
4Advantages of MMC’sAdvantages over polymer matrix composites. These include higher elastic properties; higher service temperature; insensitivity to moisture; higher electric and thermal conductivities; and better wear, fatigue, and ﬂaw resistances.The drawbacks of MMCs over PMCs include higher processing temperatures and higher densities.
6Fabrication MethodFabrication methods for MMCs are varied. One method of manufacturing them is diffusion bonding (Figure 1.28), which is used in manufacturing boron/aluminum composite parts. A ﬁber mat of boron is placed between two thin aluminum foils about 0.05 mm thick. A polymer binder or an acrylic adhesive holds the ﬁbers together in the mat. Layers of these metal foils are stacked at angles as required by the design. The laminate is ﬁrst heated in a vacuum bag to remove the binder. The laminate is then hot pressed with a temperature of about 500°C and pressure of about 35 MPa in a die to form the required machine element.
8Applications of MMC’sSpace: The space shuttle uses boron/aluminum tubes to support its fuselage frame. In addition to decreasing the mass of the space shuttle by more than 145 kg, boron/aluminum also reduced the thermal insulation requirements because of its low thermal conductivity. The mast of the Hubble Telescope uses carbon-reinforced aluminum.
9Military: Precision components of missile guidance systems demand dimensional stability — that is, the geometries of the components cannot change during use. Metal matrix composites such as SiC/aluminum composites satisfy this requirement because they have high microyield strength. In addition, the volume fraction of SiC can be varied to have a coefﬁcient of thermal expansion compatible with other parts of the system assembly.
10Transportation: Metal matrix composites are ﬁnding use now in automotive engines that are lighter than their metal counterparts. Also, because of their high strength and low weight, metal matrix composites are the material of choice for gas turbine engines.
11Ceramic Matrix Composites (CMC) Ceramic matrix composites (CMCs) have a ceramic matrix such as alumina calcium alumino silicate reinforced by ﬁbers such as carbon or silicon carbide.
12Advantages of CMC’s High strength, Hardness, High service temperature limits for ceramics,Chemical inertness, andLow density.However, ceramics by themselves have low fracture toughness. Under tensile or impact loading, they fail catastrophically.
13Reinforcing ceramics with ﬁbers, such as silicon carbide or carbon, increases their fracture toughness because it causes gradual failure of the composite. This combination of a ﬁber and ceramic matrix makes CMCs more attractive for applications in which high mechanical properties and extreme service temperatures are desired.
15Manufacturing Method of CMC One of the most common methods to manufacture ceramic matrix composites is called the hot pressing method. Glass ﬁbers in continuous tow are passed through slurry consisting of powdered matrix material, solvent such as alcohol, and an organic binder (Figure 1.31). The tow is then wound on a drum and dried to form prepreg tapes. The prepreg tapes can now be stacked to make a required laminate. Heating at about 500°C burns out the binder. Hot pressing at high temperatures in excess of 1000°C and pressures of 7 to 14 MPa follows this.
17Carbon Carbon Composites Carbon–carbon composites use carbon ﬁbers in a carbon matrix. These composites are used in very high-temperature environments of up to 3315°C, and are 20 times stronger and 30% lighter than graphite ﬁbers.
18Advantages of C-C Composites Carbon is brittle and ﬂaw sensitive like ceramics. Reinforcement of a carbon matrix allows the composite to fail gradually and also gives advantages such as ability to withstand high temperatures, low creep at high temperatures, low density, good tensile and compressive strengths, high fatigue resistance, high thermal conductivity, and high coefﬁcient of friction.Drawbacks include high cost, low shear strength, and susceptibility to oxidations at high temperatures.
20Processing a c–c composite Low-pressure carbonization A graphite cloth is taken, impregnated by resin (such as phenolic, pitch, and furfuryl ester), and laid up in layers. It is laid in a mold, cured, and trimmed. The part is then pyrolized, converting the phenolic resin to graphite. The composite is then impregnated by furfuryl alcohol. The process drives off the resin and any volatiles. The process is repeated three or four times until the level of porosity is reduced to an acceptable level. Each time, this process increases its modulus and strength. Because carbon–carbon composites oxidize at temperatures as low as 450°C, an outer layer of silicon carbide may be deposited.
22Applications of c-c composites Space shuttle nose cones: As the shuttle enters Earth’s atmosphere, temperatures as high as 1700°C are experienced.Aircraft brakes: The carbon–carbon brakes cost $970/kg, which is several times more than their metallic counterpart; however, the high durability (two to four times that of steel), high speciﬁc heat (2.5 times that of steel), low braking distances and braking times (three-quarters that of berylium), and large weight savings of up to 450 kg on a commercial aircraft such as Airbus A300-B2K and A300-B4 are attractive.
23Mechanical fasteners: Fasteners needed for high temperature applications are made of carbon–carbon composites because they lose little strength at high temperatures.
24Natural fibers NATURAL FIBERS abaca, coconut, flax, hemp, jute, kenaf and sisal are the most common — are derived from the bast or outer stem of certain plants.They have the lowest density of any structural fiber but possess sufficient stiffness and strength for some applications.The automotive industry, in particular, is using these fibers in traditionally unreinforced plastic parts and even employs them as an alternative to glass fibers. European fabricators hold the lead in use of these materials, in part because regulations require automobile components to be recyclable.
26Applications 1. Car parts Exterior body parts Car Hood Door panels Front bumpers and fendersVarious interior parts
27Natural fiber composites vs. synthetic fiber composites StudyMaterialsApplicationPerformanceSchmidt & Meyer (1998)Hemp-EPDM-PP vs. GF-EPDM-PPAuto Insulation component (Ford car)Hemp fibers are able to replace glass fibersDiener & Siehler (1999)GF-PP vs. Flax-PPAuto car panel (Mercedes A car)Successfully passed all testWotzel et al. (1999)Hemp – Epoxy vs. ABSAuto side panelDo not discuss the performanceCorbiere-Nicollier et al. (2001)China reed-PP vs. Glass-PPTransport palletSatisfying service requirementSource : Joshi et al. (2003)
28Weight Reduction Source : Joshi et al. (2003) Component Study NFRP componentBase componentAuto side panelWotzel et al.820 g (hemp-epoxy)1125 g (ABS)Auto insulationSchmidt & Meyer (1998)2.6 kg (hemp-PP)3.5 kg (GF-PP)Transport-PalletCorbiere-Nicollier et al. (2001)11.77 kg (China reed – PP)15 kg (GF – PP)Source : Joshi et al. (2003)
292. Recreation and Leisure RailingPatio furnitureDecking product
303. Insulated Roofing Roof sandwich with foam core Roof sandwich structure with bamboo core
32Mechanics Terminology The approach to analyze the mechanical behavior of composite structures is:Find the average properties of a composite ply from the individual properties of the constituents. Properties include stiffness, strength, thermal, and moisture expansion coefﬁcients. Note that average properties are derived by considering the ply to be homogeneous. This is called the micromechanics of a lamina.
33Develop the stress–strain relationships for a unidirectional/bidirectional lamina. Loads may be applied along the principal directions of symmetry of the lamina or off-axis. Also, one develops relationships for stiffness, thermal and moisture expansion coefﬁcients, and strengths of angle plies. Failure theories of a lamina are based on stresses in the lamina and strength properties of a lamina. This is called the macromechanics of a lamina.
35An isotropic material has properties that are the same in all directions. A homogeneous body has properties that are the same at all points in the body.At a point in an anisotropic material, material properties are different in all directions.A nonhomogeneous or inhomogeneous body has material properties that are a function of the position on the body.
36A lamina (also called a ply or layer) is a single ﬂat layer of unidirectional ﬁbers or woven ﬁbers arranged in a matrix.A laminate is a stack of plies of composites. Each layer can be laid at various orientations and can be made up of different material systems.
37Hybrid composites contain more than one ﬁber or one matrix system in a laminate. Interply hybrid laminates: contain plies made of two or more different composite systems.Intraply hybrid composites: consist of two or more different ﬁbers used in the same ply.An interply–intraply hybrid : consists of plies that have two or more different ﬁbers in the same ply and distinct composite systems in more than one ply.Resin hybrid laminates: combine two or more resins instead of combining two or more ﬁbers in a laminate.